|Monthly Tech-Tip |
This is the Ravenscrag Slip I used to calcine at it 1850F (about 10lbs in a bisque vessel). I am now roasting it to 1000F instead, this produces a smoother powder, less gritty. To make sure the heat penetrates for this size vessel I hold it for 2 hours at 1000F. If your container is smaller you could do less time, if any black material remains inside, then do a longer soak on the next firing. It is not actually calcining, since not all crystal water is expelled, so we call it "roasting". Why do this? Ravenscrag Slip is a clay, it shrinks. If the percentage is high enough the glaze can crack on drying (especially when applied thickly). The roast does not shrink. The idea is to tune a mix of raw and roast Ravenscrag to achieve a compromise between dry hardness and low shrinkage. Technically, Ravenscrag losses 3% of its weight on roasting so I should use 3% less. But I often swap them gram-for-gram.
This picture does not fully convey how much better the Ravenscrag is as a liner glaze (vs. G1947U). It has depth and looks much richer. It course, it could be opacified somewhat to be whiter and would still retain the surface quality (as long is it is not too opaque). The body is Plainsman H450. The outside glaze is pure Alberta Slip.
GR10-A - Pure Ravenscrag Slip
Ravenscrag all by itself makes a great cone 10 reduction semi-gloss glaze. It also has great working properties.
GR6-A - Ravenscrag Cone 6 Clear Glossy Base
This Plainsman Cone 6 Ravenscrag Slip base is just the pure material with 20% added frit to make it melt to a glossy natural clear.
Calcining is simply firing a ceramic material to create a powder of new physical properties. Often it is done to kill the plasticity or burn away the hydrates, carbonates, sulfates of a clay or refractory material.